| ||Format||Pages||Price|| |
|9||$45.00||  ADD TO CART|
|Hardcopy (shipping and handling)||9||$45.00||  ADD TO CART|
|Standard + Redline PDF Bundle||18||$54.00||  ADD TO CART|
Significance and Use
Core sampling is widely accepted, when applicable, for obtaining a laboratory sample representative of the clean wool fiber present in a lot of packaged raw wool.
If the wool is so loosely packed that a core cannot be cut, or if it is so highly compressed that the sampling tool cannot readily penetrate into the package to the required depth and in the required direction, core sampling is not applicable. The density of wool in most types of commercial packages is suitable for sampling by this method.
The procedure described in this practice is adapted to the application of statistical methods for estimating the size of sample required to achieve a required level of sample precision at minimum cost.
Note 1—The basic sampling equipment, operating procedure, and statistical approach used in this practice have been adapted for sampling lots of wool for the determination of other properties that are not affected by boring, such as average fiber diameter, and for sampling lots of other bulk fibers in packages.
1.1 This practice for sampling covers a procedure for obtaining samples from lots of grease, pulled, or scoured wool or related animal fibers in bales or bags for the determination of the clean wool fiber present by a procedure similar to that described in Test Method D584.
1.2 This practice provides a description of suitable core sampling equipment, the sampling procedure, and the method for determining the number of packages to be bored and the number of cores to be taken from each sampled package.
1.3 Reliable estimates are given for the standard deviation of the percentage clean wool fiber present between packages and within packages for lots of many types of raw wool.
1.4 The values stated in inch-pound units are to be regarded as standard. The values given in parentheses are mathematical conversions to SI units that are provided for information only and are not considered standard.
1.5 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
D123 Terminology Relating to Textiles
D584 Test Method for Wool Content of Raw Wool--Laboratory Scale
D4845 Terminology Relating to Wool
E105 Practice for Probability Sampling of Materials
E122 Practice for Calculating Sample Size to Estimate, With Specified Precision, the Average for a Characteristic of a Lot or Process
ICS Number Code 59.060.10 (Natural fibres)
UNSPSC Code 11151508(Wool fibers)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM D1060-10, Standard Practice for Core Sampling of Raw Wool in Packages for Determination of Percentage of Clean Wool Fiber Present, ASTM International, West Conshohocken, PA, 2010, www.astm.orgBack to Top